Research Inventy : International Journal of Engineering and Science is published by the group of young academic and industrial researchers with 12 Issues per year.
RESEARCH INVENTY: International Journal of Engineering and ScienceISSN: 2278-4721, Vol. 1, Issue 9 (November2012), PP 8-13www.researchinventy.com Simultaneous Extraction of Copper and Iron from Chalcopyrite Concentrates in Hydrochloric Acid Media: Effect of Additives and Temperature 1 Sampad Ghosh, 2Balram Ambade, 3Shailesh Kumar Prasad, 4Anand K. Choudhary 1,2,3,4 Chemistry Department, National Institute of Technology, Jamshedpur-831014, Jharkhand, IndiaAbstract: Studies on the chlorination of a chalcopyrite concentrate in aqueous slurry by gaseous chlorine havebeen demonstrated in this investigation. The effect of time, acid concentration, p ulp density (PD) of the sulphideconcentrate, effect of sodium chloride on dissolution of copper and the temperature of chlorination, on thefraction of copper dissolved, has been investigated. At the optimum flow rate of Cl 2 gas (400 mL min -1 ), thepercent of copper dissolved is found to be increasing with increase in acid concentration, temperature in therange of 318K to 333K and also increasing with decrease with pulp density, addition of sodium chloride,studied. The activation energy of the chlorination process has been calculated to be 7.26 kJ mol -1 . The best fit ofkinetic data to a diffusion-controlled model indicated that diffusion through the product layer was the rate -controlling step during the dissolution. At 333K, with 10wt% concentrate in the slurry and using pure Cl 2 gaswith a flow rate of 400 ml/min, nearly 93% of copper extraction has been achieved in about 1 hr. Themechanism of the leaching was further established by characterising the original concentrate and the leachresidue by XRD phase identification studies.Keywords: Chalcopyrite concentrate, Chlorine leaching, Dissolution, Hydrochloric acid, and Copper, Iron. 1. Introduction Extractive metallurgy consists of the science and art of obtaining commercial grades of metal fro m orematerial mined fro m the earth’s crust. CuFeS2 (chalcopyrite) is the most abundant primary copper ore, and as aresult, the extract ive metallurgy of copper is based largely on this mineral. A mongst the non-ferrous metalscopper is one of the most commonly used metal over thousand years. The traditional industries are continuing tosurvive and flourish due to the art of making and shaping of copper and copper alloys. Develop mental of non -conventional energy sources and the superiority of copper in solar heating are expected to dictate the use of themetal in large quantities in the near future . Chalcopyrite is the principal source fro m wh ich copper iscommercially extracted. The current practice of extracting copper from sulphidic ores su ch as chalcopyriteinvolves beneficiation through froth flotation, which produces a concentrate, followed by smelting and electro -refining to produce copper metal.In the traditional pyro metallurg ical processes, chalcopyrite concentrates aresmelted in reverberatory/flash smelters. These processes provide an energetically efficient route for theextraction of metals fro m sulphide concentrates because the sulphide sulphur is used as a fuel . Besides thepyrometallurgical methods where environmental pollution resulting emission of SO2 gas is a real problem, alsohydrometallu rgical methods are increasingly used . However, it has been established that chalcopyriterequires the presence of an oxidizing agent for its dissolution . Nu merous leaching process es have beenadvocated for recovering copper values from chalcopyrite concentrate. Conventional pyro-/hydro metallu rgicalprocess for recovery of copper from copper concentrate usually follows roasting -leaching and electrowinningsteps . Elimination of copper in the roasting step for such a system is considered most attractive from theeconomic and environmental points of view. The roasting of chalcopyrite has been an important step for theextraction of copper, in the traditional smelting route and more so in newer processes. As a result, numerousattempts have been employed to study the roasting parameters; its mechanism and the reactions involved.Elimination of copper in the roasting step for such a system is considered most attractive fro m the econom ic andenvironmental points of view. 2CuFeS2 + 7.5 O2 2CuSO4 + Fe2 O3 + 2SO2 Ho wever, it has been established that chalcopyrite requires the presence of an oxid izing agent for itsdissolution . Pressure leaching at high temperature and oxygen pressure has not found favour because ofproblems associated with the operation and maintenance of autoclaves and materials of construction [7-8].Therefore an alternative p rocess such as direct oxidative leaching is considered an impart option to addresssome of these problems [9-10]. The selection of an o xidizing agent suitable for hydrometallurgical recovery of 8
Simultaneous Extraction Of Copper And Iron From Chalcopyrite...copper fro m copper concentrate has been given considerable attention results on the direct lea ching of copperhave been reported in several processes. These processes involve ferric sulphate and ferric chloride, cupricchloride and ozone as the oxidants [11-19]. But due to the corrosive nature and difficulty in storage of chlorinegas, its use has been restricted so far . Today, with the availab ility of imp roved corrosion -resistant metalsand alloys, the use of chlorine gas as a leaching agent seems to have potential for develop ment and growth inmany specific areas of base metal extract ion and processing, dissolution kinetics of oxid ized and sulphidecopper ores in water saturated with chlorine gas been studied by many authors [21-26]. Dutrizac showed thatthe activation energy in chlorine solution is about 42 KJ / mole as co mpared to 75 KJ/ mo le in sulphate system. Palmer et al reported dissolution of chalcopyrite in chloride solution containing hydrochloric acid, sodiumchloride and ferric chloride . Lu et al studied mixed chloride sulphate leaching of chalcopyrite in acid icsolution and reported very poor leaching efficiency in absence of chloride . Groove et al achieved 90%extraction with chlorine leaching of copper sulphide minerals in an enclosed perc olation column [29-30]. In thispaper, studies on chlorine gas has been chosen as the leaching agent because leaching in chloride media is muchmore effective than sulphate system and yields high current efficiency with better quality with respect to purityduring electrolysis. Therefore the main objective of the present work is to study the leaching behaviour ofchalcopyrite mineral in chlorine media using chlorine gas and the effects of acid concentration, temperature,sodium chloride on the dissolution kinetics have been systematically investigated. 2. Experimental The chalcopyrite concentrate sample, used for this investigation was a high grade and collected fro mGhatsila, (Jharkhand, India). The material was sieved to 45m size to obtain the particle distribution andchemical analysis of the sample is incorporated in Table 1. Fe Cu Mn As Zn Ni Pb 35.18 21.80 0.01 0.002 0.045 0.003 0.001 Table 1. Chemical co mposition (%) of chalcopyrite concentrate. The material was sieved to obtain the particle size distribution. The XRD of concentrate is given inFigure 1. Hydrochloric acid and sodium chloride of laboratory reagent grade were used in this study. Analyticalgrade chemicals were used for analysis. Leaching experiments were carried out in a closed three-necked glassvessel, which was placed on a thermostatically controlled magnetic stirrer. Chemically pure Cl 2 gas stored incylinder was used in the leaching experiments. For each experiment the desired amount of copper concentratewas added to the 0.25L leaching solution containing a known amount of hydrochloric acid maintained at therequired temperature. The temperature was monitored and controlled by passing water through the bath. Atselected time intervals, a known amount of slurry s ample was withdrawn and filtered by Whatmann 41 filterpaper; copper and iron in the filtrate were analysed titrimetrically using standard methods (Vogel, 1989). Thesamples were chemically analysed for the copper and iron content percentage by atomic abso rptionspectrophotometer (AAS). The solid residue was also analysed sometimes to check the material balance.Analytical grade reagents were used for chemical analysis. Purity of the oxygen and chlorine gas used in theleaching experiments was of good quality. Phases in the concentrate, chalcopyrite ore and leach residue wereanalysed by XRD. In this manner, the dissolution of copper and iron at different periods of chlorination underthe desired experimental condit ions was determined. Figure 1. The XRD pattern of chalcopyrite concentrate used in this study . 9
Simultaneous Extraction Of Copper And Iron From Chalcopyrite... 3. Results & Discussion X-ray diffraction studies as well as petrological studies indicated the presence of chalcopyrite as the major copper and iron containing phase along with hematite and quartz in minor quantities. In the present investigation, various leaching parameters such as acid concentration, effect of sodiu m chloride and temperature with time were studied to optimise the leaching condition for dissolution of chalcopyrite. 3.1 Leaching of Chalcopyri te in Presence of Oxygen Gas Leaching of chalcopyrite in presence of oxygen gas, the effect of acid concentration, sodium chloride and temperature with time, on the extent of copper and iron present in the concentrate, has been investig ated. The results are summarised and discussed in the following pages. 3.1.1. Effect of Oxygen Leaching experiment in absence of oxygen was carried out under the condition: PD – 10%, HCl – 1.5 N at temperature of 900 C. The experimental results are presented in Fig. 2 wh ich shows very poor dissolution of both copper and iron. Dissolution of copper is nil even after 4 h of leaching where as only 18% iron gets dissolved. However, when the same experiment was repeated by passing oxygen gas, very fast dissolu tion of copper as well as iron occurs. The percentage dissolution increases with time. A maximu m of 68.2% Cu and 90.5% Fe d issolution occurs at 7 h time interval. 100 Cu with O2 90 Cu without O2 80 Fe with O2 70 % Dissolution Fe without O2 60 50 40 30 20 10 0 0 1 2 3 4 5 6 7 Time (h) Figure 2. Leaching of chalcopyrite in presence and absence of oxygen, HCl – 1.5 N, O2 flow rate 400 mL/ min, Temp. – 363K, PD - 10%. 3.1.2 Effect of Sodium Chlori de Effect of sodium chloride on chalcopyrite dissolution in hydrochloric acid was studied at 363K; 400 ml/ min o xygen flo w rate and 10% PD and the results are represented in Fig. 3 (a) & 3 (b) for copper and iron respectively. The percentage recovery increases with increase in time. Surprisingly, sodium chloride has a negative effect on chalcopyrite dissolution. The results showed copper recovery decreased from 68.2% to 46.4% by addition of 5% (w/v) of sodiu m chloride. The percentage dissolution further decreased to only 3.8% with increase in sodium chloride fro m 5% to 10% (w/v). Similar trend is also observed for iron dissolution. With addition of 5% sodium chloride iron recovery decrease from 90.5% to 79.4% at 4h duration which is further decreased to 77.4% with addition of 10% sodiu m chloride. The decrease in dissolution rate of both copper and iron may be due decrease in the solubility of o xygen during leaching . 100 70 (a) Fe : without NaCl (b) Cu : Without NaCl Fe : with 5% NaCl 60 Cu : With 5% NaCl 80 Fe : with 10% NaCl Cu : With 10% NaCl % Dissolution% Dissolution 50 60 40 30 40 20 20 10 0 0 0 1 2 3 4 0 1 2 3 4 Time (h) Time (h) Figure 3. (a) Effect of sodium chloride on copper dissolution during leaching of chalcopyrite in presence of oxygen, HCl – 3.0 N, Temp.- 363K, PD - 10%, Oxygen - 400 mL/ min. and (b) Effect of sodium chloride on iron dissolution during leaching of chalcopyrite in presence of o xygen, HCl – 3.0 N, Temp .- 363K, PD - 10%, Oxygen - 400 mL/ min. 10
Simultaneous Extraction Of Copper And Iron From Chalcopyrite...3.1.3. Effect of Temperature In the dissolution behaviour of chalcopyrite, the leaching experiments were carried out at differenttemperature between 353K and 363K. The recoveries of different metals at different time intervals are plotted inFig. 4 in the presence of 3 N hydrochloric acid, 10% sodium chloride and 400 mL/ min o xygen flow rate.Copper recovery decreases with increasing the temperature fro m 353K to 363K. At 353K recovery of copperincreased from 7.6% at 2h to 48% at 4 h duration. However with increase in leaching temperature to 363Kcopper recovery decreased from 48% to 3.8% at 4h time interval. The temperature has reverse trend for irondissolution i.e. with the increase in temperature recovery of iron is also increased. Percentage dissolutionincreased fro m 66.7% to 77.4% at 4 h duration. 80 Cu: 1.5 N HCl Cu: 3.0 N HCl 70 Fe: 1.5 N HCl 60 Fe: 3.0 N HCl % Dissolution 50 40 30 20 10 0 0 1 2 3 4 Time (h)Figure 4. Effect of temperature on copper and iron recovery fro m chalcopyrite. PD - 10%, [HCl] – 3 N, Oxygen - 400 mL/ min.3.1.4. Effect of Aci d Concentration The effect hydrochloric acid concentration on the leaching of different metal fro m the bulk sulphidewas studied using 1.5 to 3.0 N HCl and the results are presented in Fig. 5. In these experiments, the leachingtemperature 363K with oxygen flow rate of 400 ml and pulp density of 10% were maintained constant. Theresults showed that dissolution of metals increased with increase in acid concentration. However a verymarginal effect acid concentration on percentage copper recovery was observed when hydrochloric acidconcentration increased. Copper recovery increased from 2.7% to 3.8% with increase in acid concentration from1.5 N to 3 N at 4h duration. In both the cases copper dissolution is almost nil till 3 h. Increase in percentage ofiron recovery is observed with increase in time interval as well as acid concentration. Iron recovery is increasefro m 68.4% to 77.4% with increase in acid concentration fro m 1.5N to 3.0N at 4 h duration. 80 Cu at 353K 70 Cu at 363K Fe at 353K 60 Fe at 363K % Dissolution 50 40 30 20 10 0 0 1 2 3 4 Time (h)Figure 5. Effect of acid concentration on copper and iron recovery fro m chalcopyrite. PD - 10%, Temp . - 363 K, Oxygen - 400 mL/ min.3.2. Leaching in presence of chlorine g as3.2.1 Effect of Aci d Concentrati on Leaching of chalcopyrite of composition mentioned in Table 1 was carried out at 333 K by passingchlorine gas in presence absence of HCl. Ch lorine gas from the cylinder was passed in to the reaction mixtu rethrough a series of valves and rotameter. Dissolution occurs very fast with chlorine gas and a maximu m 11
Simultaneous Extraction Of Copper And Iron From Chalcopyrite... recovery of about 92% copper and 82.5% iron is achieved. Faster dissolution occurs in presence of acid as compared to dissolution in absence of acid (Fig. 6). Percentage recovery of both copper and iron increase from 80.9 and 71.4 in absence of acid to 92.7 and 82.5 respectively with 2 N HCl in 1h. 100 Cu : without HCl Cu : 2N HCl Fe : without HCl 80 Fe : 2N HCl % Dissolution 60 40 20 0 0.0 0.2 0.4 0.6 0.8 1.0 Time (h) Figure 6. Effect of acid concentration on dissolution of chalcopyrite in presence of chlorine gas. Temp. – 333 K. PD – 10%, Cl2 flow rate – 400 mL/ min . 3.2.2 Effect of Temperature Experiments on the dissolution behaviour of chalcopyrite were carried out at varying temperature between 318K and 348K in the presence of 1.0 N hydrochloric acid, and 400 mL/ min chlorine gas flow rate. The data are represented in Fig. 7 (a) for copper and in Fig. 7 (b) for iron. Copper recovery was found to be maximu m at 333K and similar leaching behaviour was obtained at temperature 318 K and 348K. Recovery of copper at 333K decreases from 82.4% to 76.5% at 318K and 70% at 348K in 1 h duration. Temperature has very marginal effect on iron dissolution in chalcopyrite with chlorine gas. Final recovery at 1 h duration increased from 71.4% to 77.8% with increase in temperature form 318K to 333K. Again iron recovery decreased to 70.6% with further increase in temperature to 348K. Decrease in chalcopyrite dissolution at higher temperature may be due to decrease in the solubility of ch lorine gas in the lixiv iant. Cu : at 318K (a) 80 (b) 80 Fe : at 318K Cu : at 333K Fe : at 333K Cu : at 348K Fe : at 348K 60 60% Dissolution % Dissolution 40 40 20 20 0 0 0.0 0.2 0.4 0.6 0.8 1.0 0.0 0.2 0.4 0.6 0.8 1.0 Time (h) Time (h) Figure 7. (a) Effect of temperature on dissolution of copper fro m chalcopyrite in presen ce of chlorine gas. [HCl].- 1.0 N. PD – 10%, Cl2 flo w rate – 400 mL/ min. and (b ) Effect of temperature on dissolution of iron fro m chalcopyrite in presence of chlorine gas. [HCl] - 1.0 N. PD – 10%, Cl2 flow rate – 400 mL/ min. 3.2.3 Effect of Sodium chl ori de Effect of sodiu m chloride on dissolution of chalcopyrite in hydrochloric acid media was studied at 333K, 400mL/ min chlorine gas flow rate, 10% PD and the results are presented in Fig. 8(a) & Fig. 8(b) for copper and iron respectively. Due to the addition of sodium chloride, it lowers the dissolution of chalcopyrite. The results showed that dissolution of metals decrease with the addition of sodium chloride. Copper recovery decreased from 82.4% to 67.7% with addition of 5% (w/v) of sodium ch loride. The percentage dissolution of copper further decreased to only 4.4% with fu rther increase of sodium ch loride fro m 5% (w/v) to 10% (w/v). Similarly with the addition of 5% (w/v) sodiu m chloride, iron recovery decreases from 77.7% to 74.3% at 1h which further decreases to 70.4% with the addition of 10% (w/v) with addition of 10% sodium chloride. The decrease in dissolution rate of both copper and iron may be due decrease in the solubility of chlorine gas in presence of sodium chloride during leaching. 12
Simultaneous Extraction Of Copper And Iron From Chalcopyrite... Cu : Without NaCl (a) Fe : without NaCl (b) 80 Cu : With 5% NaCl 80 Fe : with 5% NaCl Cu : With 10% NaCl Fe : with 10% NaCl 60 60% Dissolution % Dissolution 40 40 20 20 0 0 0.0 0.2 0.4 0.6 0.8 1.0 0.0 0.2 0.4 0.6 0.8 1.0 Time (h) Time (h) Figure 8. (a) Effect of sodium chloride on copper dissolution during leaching of chalcopyrite in presence of chlorine gas, [HCl]- 1.0 N, PD – 10%, temperature – 333K and Cl2 flo w rate – 400 mL/ min. & (b) Effect of sodium chloride on iron d issolution during leaching of chalcopyrite in presence of chlorine gas, [HCl]- 1.0 N, PD – 10%, temperature – 333K and Cl2 flow rate – 400 mL/ min. 4. Conclusion Systematic investigation on dissolution of copper and iron from chalcopyrite ore in o xygen and chlorine gas atmosphere in different react ion media, the following conclusions may be drawn fro m this study: Dissolution of copper and iron fro m chalcopyrite ore in p resence of oxygen and chlorine gas is affected in different environments like acid concentration, temperature and presence of sodium chloride.-A mount of copper and iron dissolution from chalcopyrite ore is maximu m in acidic media in both the cases in oxygen and chlorine gas environment, keeping the other parameters constant. Oxidative dissolution of chalcopyrite in presence of chlorine gas is faster than that in presence of oxygen gas. At 333 K temperature, 10% PD, 400 mL/ min. Cl2 flow rate and 2N HCl in presence of chlorine gas is an optimu m condition for leach ing. Presence of sodium chloride as a leachant decreases the rate of metal extraction fro m the chalcopyrite ore both in oxygen and chlorine med ia.The presence of chloride ions in acid ic solution enhances the format ion of porous sulfur reaction product that allows the diffusion of reactants through the product sulfur film. Acknowledgement The authors wish to express their gratitude to Dr. R. K. Jana, Dr. K. K. Sahu, National Metallu rgical Laboratory (CSIR), Jamshedpur, India, for experimental support. References 1 (a) Prasad, S.; Pandey, B.D. Minerals Engineering 1998, 11, 763-781 (b) Nahar, N.M. Renewable Energy 2002, 26(4), 623-635. 2. (a) Rabaey, K.; Clauwaert, P.; Aelterman, P.; Verstraete, W. Environ. Sci. Technol. 2005, 39, 8077-8082. (b) Lu, Z.Y.; Jeffrey, M.I.; Lawson, F. Hydrometallurgy 2000, 56, 189-202. 3. Havlik, T .; Laubertova, M.; Miskufova, A.; Kondas, J.; Vranka, F. Hydrometallurgy 2005, 77, 51-59. 4. Velásquez-Yévenes, L.; Nicol, M.; Miki, H. Hydrometallurgy 2010, 103, 108-113. 5. Pandey, A.M.; Gupta, K.N.; Altekar, V.A. Hydrometallurgy 1982, 9, 57-68. 6. Acero, P.; Cama, J.; Ayora, C.; Asta, M.P. Geologica Acta. 2009, 7(3), 389-397. 7. Owusu, G.; Dresinger, D.B. Hydrometallurgy 1995, 38, 315-324. 8. Babu, M.N.; Sahu, K.K.; Pandey, B.D. Hydrometallurgy 2002, 64, 119-129. 9. Ting-sheng, Q.; Guang-hua, N.; Jun-feng, W.; Li-feng, C. Trans. Nonferrous Met. Soc. China 2007, 17, 418-422. 10. Balaz, P.; Ebert, I. Hydrometallurgy 1991, 27, 141-150. 11. Dutrizac, J.E.; Mac Donald, W.A. Miner Sci Eng. 1974, 6, 59-100. 12. Peacey, J.; Xian-jian, G.; Robles, E. Trans. Nonferrous Met. Soc. China 2004, 14(3), 560-568. 13. Rath, P.C.; Paramguru, R.K.; Jena, P.K. Hydrometallurgy 1981, 6, 219-225. 14. Everett, P. Production of metals from minerals, International patent No. WO 94/00606, 1994. 15. Hyvarinen, Q.; Hamalainen, M. Method for producing copper in hydrometallurgical process, U.S. Patent 6,007, 600, 1999. 16. Dutrizac, J.E.; Mac Donald, R.C.; Ingraham, T.R. Trans. SME – AIME. 1969, 245, 955-959. 17. Hirato, T.; Majima, H.; Awakura, Y. Metall Trans. B. 1987, 18, 489-497. 18. Kametani, H.; Aoki, A. Metall Trans. B. 1985, 16, 695-705. 19. Havli, T.; Dvorscikova, J.; Ivanova, Z.; Kammel, R. Metallurgie 1999, 53, 57-60. 20. Ekinci, Z.; Colak, S.; Cakici, A.; Sarac, H. Materials Engineering 1998, 11, 279-283. 21. Colak, S.; Alkan, M.; Kocakerim, M. Hydrometallurgy 1987, 18, 183-193. 22. Colak, S.; Kayadeniz I.; Ceyhun, I.; Bayramoglu, M. Chimica Acta Turcica. 1993, 21, 7-16. 23. Ekmekyapar, A.; Colak, S.; Alkan, M. J. Chem. Tech. & Biotech. 1998, 43, 195-204. 24. Bayrakceken, S.; Yasar, Y.; Colak, S. Hydrometallurgy 1990, 25, 27-36. 25. Bayrakceken, S.; Yasar, Y.; Colak, S. Hydrometallurgy 1990, 25, 357-365. 26. Sarac, H.; Kocakerim, M.; Ceyhun, I. Chimica Acta Turcica. 1994, 22, 67-74. 27. Dutrizac, J.E. Metallurgical Transaction B. 1981, 12, 371-378. 28. Palmer, B.R.; Nebo, C.O.; Rau, M.F.; Fuerstenau, M.C. Metallurgical Transaction B. 1981, 12, 595-601. 29. Grooves, R.D.; Smith, P.B. Bureau of mines report on investigation, No. 7801, 1973. 30. Cao, C.H. Metallurgical Transaction B. 1987, 18, 315-323. 13